1 26 Rev.Adv.Mater.Sci. 24(2010) O. Maksimov RECENT ADVANCES AND NOVEL APPROACHES OF P-TYPE DOPING OF ZINC OXIDE Oleg Maksimov Materials Research Institute, Pennsylvania State University, University Park, PA Received: January 02, 2010 Abstract. Due to its high radiative stability and superior optoelectronic properties, such as wide direct band gap of ~3.4 ev and high exciton binding energy of ~60 mev, ZnO is considered for the fabrication of ultraviolet and visible light emitting and laser diodes, solar-blind photodetectors. Although proof-of-concept devices were already demonstrated, further progress in this area is slowed down by the difficulties of doping ZnO p-type. Here, we discuss problems associated with doping of ZnO, cover recent progress in this area, and discuss an alternative approach to increase p-type dopability via anion substitution, replacing oxygen with other group VI elements (S, Se, Te). We also propose that these anion-substituted alloys will be extremely promising for fabrication of photovoltaic devices, such as highly efficient thin film solar cells. 1. PROPERTIES AND GROWTH OF ZnO There is significant technological and scientific interest in zinc oxide (ZnO) due to its unique physical and chemical properties . It is radiatively hard wide band gap semiconductor (E G ~3.37 ev) that can be easily doped n-type. Its band gap energy can be tuned by alloying with MgO and CdO from 7.9 ev to 2.3 ev , spanning from deep ultraviolet (UV) to visible regions of the spectrum. It has a higher exciton binding energy (E b of ~60 mev) than other wide band gap semiconductors like GaN and SiC, leading to the efficient excitonic transitions at room temperature. In addition, owing to the availability of native substrates 1 and amenability to wet chemical etching, ZnO is an extremely promising material for the development of optoelectronic devices, such as Corresponding author: Oleg Maksimov, light emitting and laser diodes (LEDs and LDs) and solar-blind photo detectors, and transparent thin film transistors. ZnO nanostructures (nanoparticles, nanorods, nanobelts, etc.), which can be synthesized using inexpensive physical vapor transport techniques, were shown to be extremely promising for the application as gas sensors, due to the large surface to volume ratio , and microlasers due to the superior optical properties . Furthermore, reports of high-temperature ferromagnetism in ZnO doped with transition metals (known as dilute magnetic oxide semiconductor)  coupled with nanosecond-long spin coherence time measured at low temperatures  makes this material extremely promising for future application in spin electronics (spintronics). 2 For comparison of ZnO with other wide band gap semiconductors see Table 1. 1 Wafers with the diameter up to 4 inches are available from a number of companies including Cermet Inc., MTI Corporation, and Zn Technology Inc. 2 Use of quantum mechanical spin states associated with the charged particles to propagate information offers potential advantages over the use of charge alone, as in present-day technology. Spintronic devices, combining the advantages of magnetic metals and semiconductors, are expected to be non-volatile, versatile, fast, capable of simultaneous data storage and processing, and power efficient. They can be used in high-density data recording and storage, quantum computation, cryptography, and microelectronic.
2 Recent advances and novel approaches of p-type doping of zinc oxide 27 Table 1. Physical properties of wide band gap semiconductors. Semiconductor Crystal Structure Band gap E G (ev) at ~ 6K E b (mev) ZnO Wurzrite Direct ZnS Zincblende Direct ZnSe Zincblende Direct ZnTe Zincblende Direct GaN Wurzrite Direct H-SiC Wurzrite Indirect Table 2. Best parameters reported for ZnO films. <0002> <10-11> FWHM of band electron density electron mobility peak peak edge emission at room at room at 10K temperature temperature Units degree degree mev cm -3 cm 2 V -1 s -1 Parameter >0.01 > mev 5 x Growth PLD PLD MBE PLD PLD Technique Substrate ScAlMgO 4 ScAlMgO 4 GaN ScAlMgO 4 ScAlMgO 4 Reference [27,81] [27,81]    High crystalline quality ZnO films are successfully deposited using a number of growth platforms, including molecular beam epitaxy (MBE), chemical vapor deposition (CVD), pulsed laser deposition (PLD), and reactive sputtering. Elemental sources (Zn and ozone or oxygen plasma), ceramic targets (ZnO), and metalorganic precursors (dimethylzinc and diethylzinc) are used with equal success. The best parameters reported for the ZnO films are shown in Table 2. Some of these growth techniques, such as PLD, can be used to deposit films and device structures only on the small wafers, up to 1 inch in diameter, and are more applicable for academic research. Others, such as sputtering, are easily scalable and allow straightforward integration with modern microelectronic industry. 2. P-TYPE DOPING OF ZnO However, further progress in this area is stalled by the difficulties of doping ZnO p-type. It is generally acknowledged that high enough doping levels are difficult to achieve both due to the background n- type doping originating from the presence of H impurities , O vacancies (V O ) , and Zn interstitials (Zn i ) , and due to the large acceptor activation energies and / or low solubility of commonly used group-v (N, P, As, Sb) and group I (Li) dopants. In addition, a slow transition from p-type to n-type conductivity was observed by a number of groups. It was tentatively assigned either to the acceptor migration from the substitutional to the interstitial position and / or to the hydrogen diffusion [10,11]. In spite of these difficulties, there are reports of ZnO doped p-type with group V (N [12,13] P [14,15], As [16-20], and Sb [21,22]), and group I (Li ) elements. Co-doping with two potential acceptors (N and As)  or acceptor and donor (N and Al) [25,26] was also studied. In the case of the acceptor-donor co-doping, the improvement is believed to be primarily due to the higher solubility of the forming N-Al-N complex. A temperature modulation epitaxy technique was also applied to achieve N-doped p-type ZnO . Nitrogen-doped layers were grown followed by the deposition of thin undoped layers at quality. In addition, doping with other elements, such as Ag and Bi, was explored [28,29]. These results are summarized in Table 3. Unfortunately, most of these results were extremely challenging to reproduce and nontrivial to interpret. For example, ZnO films grown by PLD on GaAs substrates were reported to be p-type. This was explained by the As diffusion from the GaAs substrate into the ZnO layer . However, addi-
3 28 O. Maksimov Table 3. Summary of attempts to grow p-type doped ZnO films. Dopant Growth N A (cm -3 ) (cm 2 / V s) P (Ohm cm) Reference Technique N CVD 1.06x  N CVD ZnO:N remained n-type  P Diffusion ZnO:P layer was p-type  P Sputtering 1.9x x  As PLD  As Sputtering 9x  As PLD 2.4x x  As CVD 1.45x  As PLD 4x  Sb MBE 1x  Sb PLD 1.9x  Li PLD 6.04x  N + As CVD Mixed conductivity  N + Al Sputtering 2.52x  N + Al Sputtering 1.45x  N PLD 8  Ag PLD 4.9x x  Bi MBE ZnO:Bi remained n-type  tional effects, such as formation of an interfacial Zn 2 As 2 O 7 layer , Ga diffusion into the ZnO film [31,32], and Zn diffusion into the GaAs substrate  were reported by other groups. In addition, isolated As atoms should act either as deep acceptors (As is incorporated substitutionally at the O position - As O ) and donors (As is incorporated substitutionally at the Zn position - As Zn ) or remain amphoteric (As is incorporated interstitially - As i ). Thus, p-type conductivity was explained by the formation of a complex with two spontaneous Zn vacancies (As Zn -2V Zn ) . Clearly, data interpretation was not straightforward and the origin of the p-type response remained controversial. Due to the difficulties with achieving highly p-type doped ZnO, proof of concept devices that did not employ p-type ZnO layer, such as n-zno/p-srcu 2 O 2 , n-zno/p-sic , n-zno/p-si , ZnO-based metal-insulator-semiconductor , n-gan/zno nanowire/p-gan , and n-zno/p-gan were fabricated [40,41]. The last approach was widely explored due to the low lattice mismatch between ZnO and GaN and possibility of band gap engineering using Al x Ga 1-x N alloy. Thus, p-al x Ga 1-x N/ZnO/n- Mg x O LEDs operating at high temperatures, up to 650K, were demonstrated . In addition, there were a few recent reports on the fabrication of homojunction LEDs, indicating continuous progress in this area [43-47]. ZnO-based LEDs produced using spray pyrolysis were particularly promising . Possibility to use such a low-cost and easily scalable technique justifies further development of this material system. Results of these research efforts are summarized in Table 4. In addition, ZnO-based UV photo detectors - another important area of ZnO application - were demonstrated by a number of research groups [49-51]. These devices are promising for the fabrication of the early warning missile defense systems, can be used for high temperature flame detection, for the monitoring of ozone layer, and in solar astronomy. However, homojunction LEDs suffered from high turn-on-voltage, reaching 12 V in the case of Be x O-based LED, and strong deep level defect-related emission. While high turn-on-voltage can be explained by the significant resistivity of the p-type layer, deep level emission may arise due to the inferior crystalline quality of the p-type layer. Although there are reports that a large dopant concentration can be incorporated into ZnO without degradation of a crystalline quality [52,53], a poorer in-plane and out-of-plane aliment, larger tilt and twist, is often observed . This may be due both to the defects
4 Recent advances and novel approaches of p-type doping of zinc oxide 29 Table 4. Characteristics of ZnO-based LEDs. n-layer p-layer (nm) Turn-on voltage (V) Reference ZnO SrCu 2 O  ZnO:Al 4H-SiC  ZnO Si 385 Under reverse bias  ZnO 380,  GaN:Si GaN:Mg 382,  ZnO:Ga GaN:Mg  ZnO:Ga GaN:Mg  Mg x O Al y Ga 1-y N  ZnO ZnO:N Operate only below 200K  Be x O:Ga Be x O:As 363, 388,  ZnO ZnO:N 423,  ZnO ZnO:As 388,  ZnO ZnO:N  Mg x O Mg x O:N+In 450,  introduced by the dopant, such as acceptor taking interstitial position (P i, As i, Sb i ) pared with the formation of oxygen vacancy (V O ), as well as to the lower growth temperatures used to increase solubility. Therefore, a novel approach is clearly needed to achieve high crystalline quality p-type ZnO layers necessary for the fabrication of low turn-on-voltage LEDs, LDs, and p-n junction photo detectors. 4. GROWTH AND DOPING OF ANION SUBSTITUTIED ZnO It was recently suggested that p-type dopability of ZnO can be improved through the anion substitution, replacing oxygen with other group-vi elements, such as S, Se, and Te. The band alignment between ZnO and zinc chalcogenides (ZnS, ZnSe, ZnTe) is plotted in Fig. 1 . Due to the much higher valence band of zinc chalcogenides, the acceptor activation energy is lower in the anion-substituted alloys (Zn, X = S, Se, Te), making them much more amendable to p-type doping. While the cation substitution is widely used both for the band-gap engineering (Be x O, Mg x O, and Cd x O) [56-58] and for the magnetic doping (Mn x O and Co x O) [59,60], anion substitution is much less studied, with the polycrystalline films being mostly investigated [61,62]. This is particularly surprising since this approach was previously employed to overcome problem of bipolar doping in ZnSe x Te 1-x, where high p-type and n-type levels were reported for Te-rich and Se-rich alloys, respectively [63,64]. A significant success was Fig. 1. Calculated  band alignment between ZnO and zinc chalcogenides (ZnX, X = S, Se, and Te). achieved with the so-called d-doped films where p- type dopant (N) was introduced into Te-rich nanoislands embedded within the undoped ZnSe matrix. The net acceptor concentration ([N A - N D ]) ~ 18 cm -3 was achieved in the samples containing less than 3% of Te (ZnSe 0.97 Te 0.03 ) . This is an order of magnitude higher than that achieved by any other technique. There is a report on the epitaxial growth of oxide-rich Zn (y<0.15) using PLD ; on the Se-rich side up to 1.35% of oxygen were doped in ZnO y Se 1-y [67,68]. A much larger oxygen content (x<10%) was incorporated into the ZnO x Se 1-x-y
5 30 O. Maksimov Table 5. Summary of attempts to grow anion substituted ZnO alloy. Alloy Composition (%) Growth Crystalline Bowing Reference Technique Quality Parameter(eV) ZnO y S 1-y 0 < y < 100 Sputtering Polycrystalline 3  film Zn S -y 0 < y < 100 Atomic Polycrystalline 3.6  Layer film Deposition Zn S -y 0 < y < 15 PLD Epitaxial film  ZnO y Se y 0 < y < 1.35 MBE Epitaxial film  ZnO y Se y 0 < y < 1.3 MBE Epitaxial film 8  ZnO x Se 1-x-y 0 < x < 10 MBE Epitaxial film 5 - ZnOS  9 - ZnOSe Zn 0 < y < 5 Chemical Bulk crystal 3  96 < y < 100 Vapor Transport mev to 5 mev for a heavily nitrogen doped sample . With N becoming a shallow acceptor, high p- type doping levels are much easier to achieve. Fig. 2. Band gap energy plotted vs. lattice constant for selected II-VI semiconductors. Green solid lines and black dotted lines show the estimated band gaps for Me x O and ZnO y X 1-y alloys, respectively. films closely lattice matched to GaP substrates. There, epitaxial stabilization prevented phase separation . In addition, bulk Zn (y<0.05 and y>0.96) crystals were grown using chemical vapor transport technique . All these results, summarized in Table 5, indicated a significant band gap bowing. The valance band of ZnO 0.81 S 0.19 is estimated to be 410 mev higher than that of ZnO. In this case, the acceptor activation energy decreases from ANION SUBSTITUTED ZnO FOR OPTOELECTRONIC AND PHOTOVOLTAIC DEVICES It is important to note that the band gap energy of ZnO 0.81 S 0.19 remains above 3 ev. Thus, an efficient blue emission is expected from the ZnO y S 1-y - based LEDs. In addition, an enhanced photoconductivity was observed in ZnO films co-doped with Te and nitrogen . Therefore, an enhanced performance of the UV photo detectors based on the anion substituted ZnO is also expected. With the cation substitution, band gap of the Me x O (Me = Be, Mg, Cd) can be tuned from the deep UV to the visible range of spectrum. In particular, a 2.6 ev emission line (475 nm) was observed from the Zn 0.84 Cd 0.16 O films, indicating that pure green ZnO/Cd x O LEDs can be fabricated . With the anion substitution, band gap energy of the Me x can be further adjusted throughout the whole visible range (band gap of Zn x Cd 1-x O y Se 1-y can be tuned from 3.4 to 1.7 ev) down to the near-ir region of the spectrum, (band gap of CdO x Te 1-x can decrease to ~1.1 ev assuming bowing parameter of ~3 ev). We plot band gap energies versus lattice parameters for the selected II-VI semiconductors in Fig. 2. Thus, this material is extremely promising for the fabrication of full color and pure white LEDs,
6 Recent advances and novel approaches of p-type doping of zinc oxide 31 Fig. 3. The schematics of a Cd x Te y -based multi-layer graded band gap solar cell consisting of 4 layers with decreasing energy gaps (n + -window layer with E G ~ 3.4 ev, n-absorber layer, i-absorber layer, and a p-type absorber layer with E G ~ 1.5 ev). Fig. 4. The schematics of a system based on a wide band gap Me x O y X 1-y -based solar cell and an upconverter electronically isolated from each other. Up-converter consists of a tandem of two narrow band gap solar cells, such as Ge and GaAs, driving a Me x O y X 1-y -based LED. The sub-band-gap light transmitted by the wide band gap solar cell (h < E G ) is partially up-converted into high-energy photons (h > E G ), which are subsequently absorbed by the wide band gap solar cell. A reflector is located behind the up-converter to maximize collection [79,80]. where red-green-blue emission is obtained from the heterostructures that are grown on the same substrate and differ only in the composition of the quantum well region , and photovoltaic devices, in particular, for the design of the multi-layer thin film solar cells [74-76]. In these cells, a wide band gap ZnO:Ga (E G ~3.4 ev) can be used as a transparent top n-type contact, CdTe:N can be employed as a bottom p-type contact (E G ~1.5 ev), and the layers of intermediate composition can be utilized as the absorber layers, as shown in Fig. 3. Due to the compositional gradient, multi-layer solar cells will possess the gradual reduction of the band gap and the variation of electrical conduction type from n + to p + from the front to the back. The number of layers can be increased to any number in order to absorb a major part of the solar spectrum and to produce smooth slopes of energy band edges, improving the photo-generated charge carrier separation and collection. A significant improvement in efficiency is expected for these devices since two major mecha- thermalization of high-energy photons and transmis- dition, since ZnO is already considered as a transparent top contact layer in Cu(In x Ga 1-x )Se 2 -based solar cells [77,78], such a substitution will simplify device fabrication process. Moreover, Me x -based LEDs can be epitaxially integrated with the Me x -based solar cells on the top of narrow-band gap solar cells, such as Ge/GaAs multitandem structures. In this case, two narrow band gap solar cells, absorbing low energy photons, will drive LED emitting high-
7 32 O. Maksimov energy photons. These high-energy photons will be sequentially absorbed by the electrically isolated Me x -based wide band gap solar cell in addition to the photons received directly from sun, as shown in Fig. 4. A significant improvement in the efficiency predicted for such a system [79,80] makes it extremely promising for the space applications where high efficiency is of primary importance. 4. CONCLUSION In conclusion, we reviewed recent progress in the growth of ZnO-based materials and fabrication of ZnO-based devices. We covered difficulties of doping ZnO p-type, which is known as a major obstacle for the fabrication of low turn-on-voltage light emitting and laser diodes and p-n junction photo detectors. We presented and discussed novel and extremely promising approach to achieve highly p-type doped layers via anion substitution, replacing oxygen with other group-vi elements (S, Se, and Te). We also suggested that anion substituted alloys are of particular interest for the use in the photovoltaic devices, such as highly efficient thin film solar cells. REFERENCES  U. Ozgur, Y.I. Alivov, C. Liu, A. Teke, M.A. Reschikov, S. Dogan, V. Avrutin, S.J. Cho and H. Morkoc // J. Appl. Phys. 98 (2005)  J. Muth and A. Osinsky, In: Wide Bandgap Light Emitting Materials and Devices ed. by G. F. Neumark, I. L. Kuskovsky and H. Jiang (Wiley-VCH, 2007).  B.S. Kang, H.T. Wang, L.C. Tien, F. Ren, B.P. Gila, D.P. Norton, C.R. Abernathy, J. Lin and S. J. Pearton // Sensors 6 (2006) 643.  A.B. Djurisic and Y.H. Leung // Small 2 (2006) 944.  R. Janisch, P. Gopal and N. Spaldin // J. Phys.: Condens. Matter 17 (2005) 657.  S. Ghosh, V. Sih, W.H. Lau, D. D. Awschalom, S.Y. Bae, S. Wang, S. Vaidya and G. Chapline // Appl. Phys. Lett. 86 (2007)  C.G. Van de Walle // Phys. Rev. Lett. 85 (2000)  E.C. Lee, Y.S. Kim, Y.G. Jin and K. J. Chang // Phys. Rev. B 64 (2001)  A.F. Kohan, G. Ceder, D. Morgan and C.G. Van de Walle // Phys. Rev. B 61 (2000)  L.G. Wanf and A. Zunger // Phys. Rev. Lett. 90 (2003)  T.M. Barnes, K. Olson and C.A. Wolden // Appl. Phys. Lett. 86 (2005)  X. Li, Y. Yan, T.A. Gessert, C. DeHart, C.L. Perkins, D. Young and T.J. Coutts // Electrochemical and Solid-State Lett. 6 (2003) 56.  Z.Q. Fang, B. Claflin, D.C. Look, L.L. Kerr and X. Li // J. Appl. Phys. 102 (2007)  S. Jang, J.J. Chen, B.S. Kang, F. Ren, D.P. Norton, S.J. Pearton, J. Lopata and W.S. Hobson // Appl. Phys. Lett. 87 (2005)  Z.G. Yu, P. Wu and H. Gong // Appl. Phys. Lett. 88 (2006)  Y.R. Ryu, S. Zhu, D.C. Look, J.M. Wrobel, H.M. Jeong and H.W. White // J. Crystal Growth 216 (2000) 330.  D.C. Look, G.M. Renlund, R.H. Burgener and J.R. Sizelove // Appl. Phys. Lett. 85 (2004)  V. Vaithinathan, B.T. Lee, C.W. Chang, K. Asokan and S.S. Kim // Appl. Phys. Lett. 88 (2006)  J.C. Sun, J.Z. Zhao, H.W. Liang, J.M. Bian, L.Z. Hu, H.Q. Zhang, X.P. Liang, W.F. Liu and G.T. Du // Appl. Phys. Lett. 90 (2007)  C. Yuen, S.F. Yu, E.S.P. Leong, S.P. Lau, K. Pita, H.Y. Yang and T.P. Chen // J. Appl. Phys. 101 (2007)  L.J. Mandalapu, Z. Yang, F.X. Xiu, D.T. Zhao and J.L. Liu // Appl. Phys. Lett. 88 (2006)  W. Guo, A. Allenic, Y.B. Chen, X.Q. Pan, Y. Che, Z.D. Hu and B. Liu // Appl. Phys. Lett. 90 (2007)  J.G. Lu, Y.Z. Zhang, Z.Z. Ye,Y. J. Zeng, H.P. He, L.P. Zhu, J.Y. Huang, L. Wang, J. Yuan, B.H. Zhao and X.H. Li // Appl. Phys. Lett. 89 (2006)  A. Krtschil, A. Dadgar, N. Oleynik, J. Blasing, A. Diez and A. Krost // Appl. Phys. Lett. 87 (2005)  G. Lu, Z.Z. Ye, F. Zhuge, Y.J. Zeng, B.H. Zhao and L.P. Zhu // Appl. Phys. Lett. 85 (2004)  J.G. Lu, Z.Z. Ye, G.D. Yuan, Y.J. Zeng, F. Zhuge, L.P. Zhu, B.H. Zhao and S.B. Zhang // Appl. Phys. Lett. 89 (2006)  A. Tsuzazaki, A. Ohtomo, T. Ohtomo, T. Onuma, M. Ohtani, T. Makino, M. Sumiya, K. Ohtani, S.F. Chichibu, S. Fuke,
8 Recent advances and novel approaches of p-type doping of zinc oxide 33 Y. Segawa, H. Ohno, H. Koinuma and M. Kawasaki // Nature Materials 4 (2005) 42.  H.S. Kang, B.D. Ahn, J.H. Kim, G.H. Kim, S.H. Lim, H.W. Chang and S.Y. Lee // Appl. Phys. Lett. 88 (2006)  F.X. Xiu, L.J. Mandalapu, Z. Yang, J.L. Li, G. F. Liu and J.A. Yarmoff // Appl. Phys. Lett. 89 (2006)  D.J. Rogers, F.H. Teherani, T. Monteiro, M. Soares, A. Neves, M. Carmo, S. Pereira, M.R. Correia, A. Lusson, E. Alves, N.P. Barradas, J.K. Morrod, K.A. Prior, P. Kung, A. Yasan and M. Razeghi // Phys. Stat. Sol. C 3 (2006)  M.K. Ryu, S.H. Lee, M.S. Jang, G.N. Panin and T.W. Kang // J. Appl. Phys. 92 (2002) 154.  H.F. Liu, S.J. Chua, G.X. Hu, H. Gong and N. Xiang // J. Appl. Phys. 102 (2007)  S. Yu. Yuldashev, G.N. Panin, S.W. Choi, V.Sh. Yalishev, L.A. Nosova, M.K. Ryu, S. Lee, M.S. Jang, K.S. Chung and T.W. Kang // Jpn. J. Appl. Phys. 42 (2003)  S. Limpijumnong, S.B. Zhang, S.H. Wei and C.H. Park // Phys. Rev. Lett. 92 (2004)  H. Ohta, M. Orita, M. Hirano and H. Hosono // J. Appl. Phys. 89 (2001)  C. Yuen, S.F. Yu, S.P. Lau, Rusli and T.P. Chen // Appl. Phys. Lett. 86 (2005)  P. Chen, X. Ma and D. Yang // J. Appl. Phys. 101 (2007)  D.K. Hwang, M.S. Oh, J.H. Lim, Y.S. Choi and S.J. Park // Appl. Phys. Lett. 91 (2007)  S.J. Ahn and G.C. Yi // Appl. Phys. Lett. 91 (2007)  Y.I. Alivov, J.E. Van Nostrand, D.C. Look, M.V. Chukichev and B.M. Ataev // Appl. Phys. Lett. 83 (2003)  D.J. Rogers, F.H. Teherani, A. Yasan, K. Minder, P. Kung and M. Razeghi // Appl. Phys. Lett. 88 (2006)  J.W. Osinsky, M.Z. Dong, B. Kauser, A. Hertog, M. Dabiran, P.P. Chow, S.J. Pearton, O. Lopatiuk and L. Chernyak // Appl. Phys. Lett. 85 (2004)  S.J. Jiao, Z.Z. Zhang, Y.M. Lu, D.Z. Shen, B. Yao, J.Y. Zhang, B.H. Li, D.X. Zhao, X.W. Fan and Z.K. Tang // Appl. Phys. Lett. 88 (2006)  Y. Ryu, T. Lee, J.A. Lubdugan, H.W. White, B.J. Kim, Y.S. Park and C.J. Youn // Appl. Phys. Lett. 88 (2006)  Z.Z. Zhang, Z.P. Wei, Y.M. Lu, D.Z. Shen, B.Yao, B.H. Li, D.X. Zhao, J.Y. Zhang, X.W. Fan and Z.K. Tang // J. Crystal Growth 301 (2007) 362.  J.C. Sun, J.Z. Zhao, H.W. Liang, J.M. Bian, L.Z. Hu, H.Q. Zhang, X.P. Liang, W.F. Liu and G.T. Du // Appl. Phys. Lett. 90 (2007).  A. Tsuzazaki, A. Ohtomo, T. Ohtomo, T. Onuma, M. Ohtani, T. Makino, M. Sumiya, K. Ohtani, S.F. Chichibu, S. Fuke, Y. Segawa, H. Ohno, H. Koinuma and M. Kawasaki // Nature Materials 4 (2005) 42.  J. Bian, W. Liu, H. Liang, L. Hu, J. Sun, Y. Luo and G. Du // Chem. Phys. Lett. 430 (2006) 183.  W. Yang, R.D. Vispute, S. Choopun, R.P. Sharma, T. Venkatesan and H. Shen // Appl. Phys. Lett. 78 (2001)  W. Yang, S.S. Hullavarad, B. Nagaraj, I. Takeuchi, R.P. Sharma, T. Venkatesan, R.D. Vispute and H. Shen // Appl. Phys. Lett. 82 (2003)  K.W. Liu, J.Y. Zhang, J.G. Ma, D.Y. Jiang, Y.M. Lu, B. Yao, B.H. Li, D.X. Zhao, Z.Z. Zhang and D.Z. Shen // J. Phys. D 40 (2007)  K. Tamura, A. Ohtomo, K. Saikusa, Y. Osaka, T. Makino, Y. Segawa, M. Sumiya, S. Fuke, H. Koinuma and M. Kawasaki // J. Crystal Growth 214 (2000) 59.  B.J. Kwon, H.S. Kwack, S.K. Lee, Y.H. Cho, D.K. Hwang and S.J. Park // Appl. Phys. Lett. 91 (2007)  W. Guo, A. Allenic, Y.B. Chen, X.Q. Pan, Y. Che, Z.D. Hu and B. Liu // Appl. Phys. Lett. 90 (2007)  S.H. Wei and A. Zunger // Appl. Phys. Lett. 72 (1998)  Y.R. Ryu, T.S. Lee, J.A. Lubguban, A.B. Corman, H.W. White, J.H. Leem, M.S. Han, Y.S. Park, C.J. Youn and W.J. Kim // Appl. Phys. Lett. 88 (2006)  A. Ohtomo, M. Kawasaki, T. Koida, K. Masubuchi, H. Koinuma, Y. Sakurai, Y. Yoshida, T. Yasuda and Y. Segawa // Appl. Phys. Lett. 72 (1998)  S.Y. Lee, Y. Li, J.S. Lee, J.K. Lee, M. Nastasi, S.A. Crooker, Q.X. Jia, H.S. Kang and J.S. Kang // Mat. Res. Soc. Symp. Proc. 764 (2003) 413.
9 34 O. Maksimov  Z. Jin, M. Murakami, T. Fukumura, Y. Matsumoto, A. Ohtomo, M. Kawasaki and H. Koinuma // J. Crystal Growth 214 (2000) 55.  T. Fukumura, Z. Jin, A. Ohtomo, H. Koinuma and M. Kawasaki // Appl. Phys. Lett. 75 (1999)  B.K. Meyer, A. Polity, B. Farangis, Y. He, D. Hasselkamp, T. Kramer and C. Wang // Appl. Phys. Lett. 85 (2004)  C. Persson, C. Platzer-Bjorkman, J. Malmstrom, T. Torndahl and M. Edoff // Phys. Rev. Lett. 97 (2006)  W. Lin, B.X. Yang, S.P. Guo, A. Elmoumni, F. Fernandez and M.C. Tamargo // Appl. Phys. Lett. 75 (2007)  M. Strassburg, M. Strassburg, O. Schulz, U. Pohl, A. Hoffmann, D. Bimberg, A. Kontos and Y. Raptis // J. Crystal Growth 248 (2003) 50.  I.L. Kuskovsky, Y. Gu, Y. Gong, H.F. Yan, J. Lau, I.C. Noyan, G.F. Neumark, O. Maksimov, X. Zhou, M.C. Tamargo, V. Volkov, Y. Zhu and L. Wang // Phys. Rev. B 73 (2006)  Y.Z. Yoo, Z.W. Jin, T. Chikyow, T. Fukumura, M. Kawasaki and H. Koinuma // Appl. Phys. Lett. 81 (2002)  W. Shan, W. Walukiewicz, J.W. Ager III, K.M. Yu, J. Wu, E.E. Haller, Y. Nabetani, T. Mukawa, Y. Ito and T. Matsumoto // Appl. Phys. Lett. 83 (2003) 299.  Y. Nabetani, T. Mukawa, Y. Ito, T. Kato and T. Matsumoto // Appl. Phys. Lett. 83 (2003)  Y. Nabetani, Y. Ito, K. Kamisawa, T. Kato, T. Matsumoto and T. Hirai // Phys. Stat. Sol. C 3 (2006)  S. Locmelis, C. Brunig, M. Binnewies, A. Borger, K.D. Becker. T. Homann and T. Bredow // J. Mater. Sci. 42 (2007)  H.L. Porter, A.L. Cai, J.F. Muth and J. Narayan // Appl. Phys. Lett. 86 (2005)  I.A. Buyanova, J.P. Bergman, G. Pozina, W.M. Chen, S. Rawal, D.P. Norton, S.J. Pearton, A. Osinsky and J.W. Dong // Appl. Phys. Lett. 90 (2007)  Y. Luo, S.P. Guo, O. Maksimov, M.C. Tamargo, V. Asnin, F.H. Pollak and Y.C. Chen // Appl. Phys. Lett. 77 (2000)  N.B. Chaure, A.P. Samantilleke, R.P. Burton, J. Young and I.M. Dharmadasa // Thin Solid Films 472 (2005) 212.  I.M. Dharmasada // Solar Energy Materials & Solar Cells 85 (2005) 293.  I.M. Dharmadasa, J.S. Roberts and G. Hill // Solar Energy Materials & Solar Cells 88 (2005) 413.  F.J. Haug, M. Krejci, H. Zogg, A.N. Tiwari, M. Kirsch and S. Siebentritt // Thin Solid Films 361 (2000) 239.  P.J. Rostan, J. Mattheis, G. Bilger, U. Rau and J.H. Werner // Thin Solid Films 480 (2005) 67.  T. Trupke, M.A. Green and P. Wurfel // J. Appl. Phys. 92 (2002)  P. Wurfel, Physics of Solar Cells (Wiley- VCH, New York, 2007).  A. Ohtomo, K. Tamura, K. Saikusa, K. Takahashi, T. Makino, Y. Segawa, H. Koinuma and M. Kawasaki // Appl. Phys. Lett. 75 (1999)  H.J. Ko, Y.F. Chen, T. Yao, K. Miyajima, A. Yamamoto and T. Goto // Appl. Phys. Lett. 77 (2000) 537.
The study of deep-level emission center in ZnO films grown on c-al 2 O 3 substrates Guotong Du Yuantao Zhang, Jinzhong Wang, Yongguo Cui (College of Electronic Science and Engineering, State Key Laboratory
Claim#:021914-174 Initials: J.T. Last4SSN: 6996 DOB: 5/3/1970 Crime Date: 4/30/2013 Status: Claim is currently under review. Decision expected within 7 days Claim#:041715-334 Initials: M.S. Last4SSN: 2957
Epitaxy Epitaxial Growth Epitaxy means the growth of a single crystal film on top of a crystalline substrate. For most thin film applications (hard and soft coatings, optical coatings, protective coatings)
High Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures ARGYRIOS C. VARONIDES Physics and EE Department University of Scranton 800 Linden Street, Scranton PA, 18510 United States Abstract:
Lecture 19: Solar cells Contents 1 Introduction 1 2 Solar spectrum 2 3 Solar cell working principle 3 4 Solar cell I-V characteristics 7 5 Solar cell materials and efficiency 10 1 Introduction Solar cells
Solid State Detectors = Semi-Conductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the p-n junction Charge collection
MMIC Design and Technology Fabrication of MMIC Instructor Dr. Ali Medi Substrate Process Choice Mobility & Peak Velocity: Frequency Response Band-Gap Energy: Breakdown Voltage (Power-Handling) Resistivity:
CMOS Processing Technology Silicon: a semiconductor with resistance between that of conductor and an insulator. Conductivity of silicon can be changed several orders of magnitude by introducing impurity
The fabrication of a monolithic transistor includes the following steps. 1. Epitaxial growth 2. Oxidation 3. Photolithography 4. Isolation diffusion 5. Base diffusion 6. Emitter diffusion 7. Contact mask
1.5 Light absorption by solids Bloch-Brilloin model L e + + + + + allowed energy bands band gaps p x In a unidimensional approximation, electrons in a solid experience a periodic potential due to the positively
Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge
LED Review Questions 1. Consider two samples in the form of powders: sample A is a physical mixture comprising equal moles of pure Ge and pure Si; sample B is a solid solution of composition Si0.5Ge0.5.
Module 3 : Fabrication Process and Layout Design Rules Lecture 12 : CMOS Fabrication Technologies Objectives In this course you will learn the following Introduction Twin Well/Tub Technology Silicon on
GaN based Blue Laser diode ECE 355 presentation Seiyon Kim Dept. of ECE and Microelectronics Lab Outline -Motivation: Why we need BLUE lasers? -Material property: GaN vs. other wide bandgap materials -Growth
An Accurate Method for Measuring Activation Energy Xiang-Bai Chen*, Jesse Huso, John L. Morrison, and Leah Bergman Department of Physics, University of Idaho, Moscow, ID 83844-0903 Abstract In this letter,
Module 6 : PHYSICS OF SEMICONDUCTOR DEVICES Lecture 34 : Intrinsic Semiconductors Objectives In this course you will learn the following Intrinsic and extrinsic semiconductors. Fermi level in a semiconductor.
Analog & Digital Electronics Course No: PH-218 Lecture 1: Semiconductor Materials Course Instructors: Dr. A. P. VAJPEYI Department of Physics, Indian Institute of Technology Guwahati, India 1 Semiconductors
Chemical Vapor Deposition Physical Vapor Deposition (PVD) So far we have seen deposition techniques that physically transport material from a condensed phase source to a substrate. The material to be deposited
Background Story of the Invention of Efficient Blue InGaN Light Emitting Diodes SHUJI NAKAMURA SOLID STATE LIGHTING AND ENERGY ELECTRONICS CENTER MATERIALS AND ECE DEPARTMENTS UNIVERSITY OF CALIFORNIA,
Diode Applications This chapter teaches the employment of pn-junction diodes in various applications. Rectifier diodes Rectifier diodes are used, for example, in power supplies, AC-to-DC converters, and
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
Optica Applicata, Vol. XXXVII, No. 4, 2007 The study of structural and optical properties of TiO 2 :Tb thin films AGNIESZKA BORKOWSKA, JAROSLAW DOMARADZKI, DANUTA KACZMAREK, DAMIAN WOJCIESZAK Faculty of
Nanoparticle Enhanced Thin Film Solar Cells Solar Cells Solar cells convert visible light to electricity. It is one of the clean sources of energy. In theory a 100 square mile area covered with solar panels
Effect of the oxide film formed on the electrical properties of Cu-Zn alloy electric contact material Hao-Long Chen *, Ke-Cheng Tseng and Yao-Sheng Yang Department of Electronic Engineering, Kao Yuan University,
The Diode The diode is a two terminal semiconductor device that allows current to flow in only one direction. It is constructed of a P and an N junction connected together. Diode Operation No current flows
10p PhD Course Semiconductor Physics 18 Lectures Nov-Dec 2011 and Jan Feb 2012 Literature Semiconductor Physics K. Seeger The Physics of Semiconductors Grundmann Basic Semiconductors Physics - Hamaguchi
Rev.Adv.Mater.Sci. Nanostructured ZnO 10 and (2005) ZAO 335-340 transparent thin films by sputtering surface characterization 335 NANOSTRUCTURED ZnO AND ZAO TRANSPARENT THIN FILMS BY SPUTTERING SURFACE
AN OVERVIEW Semiconductors form the active regions of \intelligent" devices. The following gures provide an overview of why semiconductors are important, what the various demands in semiconductor technologies
CVD synthesis of graphene and 2D Transition metal dichalcogenides R E Beissenov 1,2, A T Galin 1, D A Muratov 1,2 and Z A Mansurov 1 1 Institute of Combustion Problems, Almaty, Kazakhstan 2 Institute of
Optical Hyperdoping: Transforming Semiconductor Band Structure for Solar Energy Harvesting 3G Solar Technologies Multidisciplinary Workshop MRS Spring Meeting San Francisco, CA, 5 April 2010 Michael P.
Solar Photovoltaic (PV) Cells A supplement topic to: Mi ti l S Micro-optical Sensors - A MEMS for electric power generation Science of Silicon PV Cells Scientific base for solar PV electric power generation
International Journal of Nanoscience Vol. 10, No. 1 (2011) 1 5 #.c World Scienti c Publishing Company DOI: 10.1142/S0219581X11007697 ROOM TEMPERATURE FERROMAGNETISM IN Co-DOPED ZnO NANOPARTICLES: MILLING
Applied Quantum Mechanics for Electrical Engineers Workshop II Energy Band Model and Doping 95 pts Objective: Explore the effect of doping on the energy band diagram and the carrier concentration. Instructions:
Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!
Photovoltaic effect for narrow-gap Mott Insulators Efstratios Manousakis Florida State University What is wrong with a band semiconductor The average energy range of the incident photon is 0.5 ev-3.5 ev.
ECE 331: Introduction to Materials for Electrical Engineers Course Objective... Introduce fundamental concepts in Materials Science and how they are used in ECE You will learn about: material structure
1 Layer Deposition: Thermal Oxidation and CVD Rupesh Gupta IIT Delhi Supervisor: Dr. Chacko Jacob 2 OUTLINE Thermal Oxidation and Model o Factors Affecting Kinetics o Future Trends: Oxidation o CVD and
Materials Science and Engineering B 106 (2004) 300 304 Fabrication of ITO thin films by filtered cathodic vacuum arc deposition B.J. Chen, X.W. Sun, B.K. Tay School of Electrical and Electronic Engineering,
contamination analysis for compound semiconductors ANALYTICAL SERVICES B u r i e d d e f e c t s, E v a n s A n a l y t i c a l g r o u p h e l p s y o u C O N T R O L C O N T A M I N A T I O N Contamination
USING MERCURY PROBES TO CHARACTERIZE USJ LAYERS James T.C. Chen and Wei Liu Four Dimensions, Inc. Hayward, CA 94545 It is well established that uniformity and dosage of drain-source ion implantation on
Blue Lasers Photonics and Optical Communications Zubin Advantages of blue lasers and Blue (GaN) LEDs are around 100 times brighter than conventional LEDs More efficient (energy-wise) than light bulbs Longer
Production of Solar Energy Using Nanosemiconductors 1 Kiruthika S, 2 Dinesh Kumar M, 3 Surendar.A 1, 2 II year, KSR College of Engineering, Tiruchengode, Tamilnadu, India 3 Assistant Professor, KSR College
A Low-Cost Carbon-Based Oxygen Electrode for Polymer Membrane Fuel Cells Dr. Qiong Cai Department of Chemical and Process Engineering, University of Surrey Email: firstname.lastname@example.org Challenges of Oxygen
Electronic Structure and the Periodic Table Learning Outcomes (a) Electronic structure (i) Electromagnetic spectrum and associated calculations Electromagnetic radiation may be described in terms of waves.
Lecture 11d Light Emitting Diodes and Laser Diodes Reading: (Cont d) Notes and Anderson 2 Chapter 11.3-11.4.5 Some images from Anderson and Anderson text Optical Design Choices Some semiconductor materials
Orientation Control Technology Using PVD for Al/TiN/Ti Layers in Al Interconnect Fabrication Se-Ju Lim*, Johji Hiroishi* and Yoshiyuki Kadokura* Interconnect materials for advanced memory devices are actively
Experimental Determination of Planck s Constant Ryan Eagan The Pennsylvania State University University Park, Pennsylvania 16802 Email: email@example.com July 25, 2011 Abstract Experimental determination
Basic types of solid materials. Overview The theory of bands provides a basis for understanding the classification and physical properties of solid materials such as electrical conductivity, optical behavior
Experimental Observation of the Quantum Anomalous Hall Effect in a Magnetic Topological Insulator Chang et al., Science 340, 167 (2013). Joseph Hlevyack, Hu Jin, Mazin Khader, Edward Kim Outline: Introduction:
Polysilicon Renewable Energy Corporation L. Carnel Scanwafer Wafers Cells Modules HIT = Heterojunction with Intrinsic Thin-layer : first used by Sanyo in 1992 and now used for high-efficiency solar cells
Chapter 5 5.6 Doped GaAs Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. Second Edition ( 2001 McGraw-Hill) b. In a sample containing only 10 15 cm -3 ionized
Semiconductor lasers and LEDs read Agrawal pp. 78-116 Objectives, understand the following: Stimulated emission, spontaneous emission, and absorption in semiconductors Design of an LED and laser diode:
Plasmonic Photovoltaic Justus C. Ndukaife, Arthur Teng Solar Power Current world consumption of electric energy is around 12 13 TW. The Earth receives more solar energy in one hour than the energy used
Materials Science-Poland, Vol. 22, No. 2, 2004 The effect of film thickness on physical properties of fluorine-doped indium oxide thin films S. M. ROZATI *, T. GANJ Physics Department, University of Guilan,
9 Solar Cell Parameters and Equivalent Circuit 9.1 External solar cell parameters The main parameters that are used to characterise the performance of solar cells are the peak power P max, the short-circuit
How MOCVD Works Deposition Technology for Beginners Contents MOCVD for Beginners...3 MOCVD A Definition...4 Planetary Reactor Technology...5 Close Coupled Showerhead Technology...6 AIXTRON MOCVD Production
Control of r. f. nitrogen plasma source in solid source MBE Courtesy of Yoon Soon Fatt. Used with permission. Mass Flow Controller Ultra High Vacuum Leak Valve RF nitrogen N 2 Gas Ultra Pure Four channel
Semiconductor doping Si solar Cell Two Levels of Masks - photoresist, alignment Etch and oxidation to isolate thermal oxide, deposited oxide, wet etching, dry etching, isolation schemes Doping - diffusion/ion
April. 15, 2010 Due April. 29, 2010 Project 2B Building a Solar Cell (2): Solar Cell Performance Objective: In this project we are going to experimentally measure the I-V characteristics, energy conversion
4.1 SOLAR CELL OPERATION Y. Baghzouz ECE Department UNLV SOLAR CELL STRUCTURE Light shining on the solar cell produces both a current and a voltage to generate electric power. This process requires a material
OPTOELECRONIC DEVICES Optoelectronic Devices - the electronic technology in which optical radiation is emitted, modified, or converted (as in electrical-to-optical or optical-toelectrical). Related technologies:
The Physics of Energy sources Renewable sources of energy Solar Energy B. Maffei Bruno.firstname.lastname@example.org Renewable sources 1 Solar power! There are basically two ways of using directly the radiative
Electronic Materials Devices and Fabrication Layering: Thermal Oxidation Dr. S. Parasuraman Department of Metallurgical and Materials Engineering Indian Institute of Technology, Madras Module - 01 Lecture
Electronic Stability & Periodic Table Things at higher energy are less stable!! All living things are dependent on their ability to acquire energy from unstable things! The compounds in the food you eat
Photovoltaic and Photoelectrochemical Solar Cells EDDIE FOROUZAN, PH.D. ARTIN ENGINEERING AND CONSULTING GROUP, INC. 7933 SILVERTON AVE. #715 SAN DIEGO, CA 92128 PSES San Diego Chapter 2012-02-10 History
Digital VLSI design Lecture 2: Complementary Metal Oxide Semiconductor (CMOS) Chips What will we learn? How integrated circuits work How to design chips with millions of transistors Ways of managing the
Applied Physics of solar energy conversion Conventional solar cells, and how lazy thinking can slow you down Some new ideas *************************************************************** Our work on semiconductor
Applied Surface Science 186 2002) 453±457 Exploring the deposition of oxides on silicon for photovoltaic cells by pulsed laser deposition Lianne M. Doeswijk a,*, Hugo H.C. de Moor b, Horst Rogalla a, Dave
UNDERSTANDING THE LIMITS OF SEMICONDUCTOR TECHNOLOGY Department of Electronic Engineering UPC, Barcelona, Spain OUTLINE OF THE COURSE Introduction and motivation Limits of the technology at fundamental,
1 Photovoltaics Photovoltaic (PV) materials and devices convert sunlight into electrical energy, and PV cells are commonly known as solar cells. Photovoltaics can literally be translated as light-electricity.
Surface and Coatings Technology 158 159 (2002) 247 252 Study on the early stage of thin filmgrowth in pulsed beamdeposition by kinetic Monte Carlo simulation a, b Q.Y. Zhang *, P.K. Chu a State Key Laboratory